#------------------------------------------------------------------------------
#$Date: 2016-03-23 23:57:12 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179519 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/16/4341656.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4341656
loop_
_publ_author_name
'Treadwell, LaRico J'
'Watkins-Curry, Pilanda'
'McAlpin, Jacob D.'
'Rebar, Drew J.'
'Hebert, Jessica K.'
'DiTusa, John F.'
'Chan, Julia Y.'
_publ_section_title
;
 Investigation of Mn, Fe, and Ni Incorporation in CeCo2Al8.
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              963
_journal_page_last               968
_journal_paper_doi               10.1021/ic502356t
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'Al8 Ce Co Fe'
_chemical_formula_sum            'Al8 Ce Co Fe'
_chemical_formula_weight         470.7525
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           55
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2014-09-13 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.4591(5)
_cell_length_b                   14.3798(6)
_cell_length_c                   4.02410(10)
_cell_measurement_temperature    298(2)
_cell_volume                     720.96(5)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Crystal Maker'
_computing_publication_material  Publcif
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'Direct Methods, SIR 97'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker Kappa D8 Quest CMOS'
_diffrn_measurement_method       'φ scan'
_diffrn_radiation_source         'I\mS microfocus tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0422
_diffrn_reflns_av_sigmaI/netI    0.0235
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            11930
_diffrn_reflns_theta_full        30.45
_diffrn_reflns_theta_max         30.45
_diffrn_reflns_theta_min         2.83
_exptl_absorpt_coefficient_mu    11.336
_exptl_absorpt_correction_T_max  0.522
_exptl_absorpt_correction_T_min  0.323
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS(2014)
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.331
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Fragment
_exptl_crystal_F_000             858.8
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.417
_refine_diff_density_min         -1.923
_refine_diff_density_rms         0.296
_refine_ls_extinction_coef       0.0225(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.247
_refine_ls_matrix_type           full
_refine_ls_number_parameters     74
_refine_ls_number_reflns         1237
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.247
_refine_ls_R_factor_all          0.0244
_refine_ls_R_factor_gt           0.0211
_refine_ls_shift/su_max          0.007
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0239P)²+0.5008P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0492
_refine_ls_wR_factor_ref         0.0512
_reflns_number_gt                1137
_reflns_number_total             1240
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            ic502356t_si_005.cif
_cod_data_source_block           scd0003
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4341656--4341665.cif.
;
_cod_original_sg_symbol_H-M      Pbam
_cod_database_code               4341656
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x-1/2, -y-1/2, z'
'-x-1/2, y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ce1 Ce 0.340544(12) 0.318648(12) 0.0000 0.00855(9) Uani 1 2 d S
Co2 Co 0.15020(3) 0.09724(3) 0.0000 0.00581(16) Uani 0.29(5) 2 d SP
Fe2 Fe 0.15020(3) 0.09724(3) 0.0000 0.00581(16) Uani 0.72(6) 2 d SP
Co1 Co 0.03460(3) 0.40615(3) 0.0000 0.00687(15) Uani 0.68(4) 2 d SP
Fe1 Fe 0.03460(3) 0.40615(3) 0.0000 0.00687(15) Uani 0.30(4) 2 d SP
Al8 Al 0.0000 0.5000 0.5000 0.0071(2) Uani 1 4 d S
Al9 Al 0.0000 0.0000 0.0000 0.0077(2) Uani 1 4 d S
Al2 Al 0.15966(6) 0.37884(7) 0.5000 0.00741(19) Uani 1 2 d S
Al5 Al 0.45229(7) 0.17998(6) 0.5000 0.00733(18) Uani 1 2 d S
Al3 Al 0.23543(7) 0.17269(6) 0.5000 0.00767(18) Uani 1 2 d S
Al4 Al 0.33146(7) 0.49203(7) 0.5000 0.00750(18) Uani 1 2 d S
Al1 Al 0.02542(7) 0.13185(6) 0.5000 0.00673(17) Uani 1 2 d S
Al7 Al 0.33860(6) 0.04479(7) 0.0000 0.0094(2) Uani 1 2 d S
Al6 Al 0.09522(6) 0.25318(5) 0.0000 0.00754(18) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al1 Ce1 Al1 79.69(2) 7_665 7_664
Al1 Ce1 Al2 150.90(3) 7_665 1_554
Al1 Ce1 Al2 93.060(18) 7_664 1_554
Al1 Ce1 Al2 93.060(18) 7_665 .
Al1 Ce1 Al2 150.90(3) 7_664 .
Al2 Ce1 Al2 79.62(2) 1_554 .
Al1 Ce1 Al5 103.18(2) 7_665 1_554
Al1 Ce1 Al5 53.93(2) 7_664 1_554
Al2 Ce1 Al5 94.716(17) 1_554 1_554
Al2 Ce1 Al5 153.95(2) . 1_554
Al1 Ce1 Al5 53.93(2) 7_665 .
Al1 Ce1 Al5 103.18(2) 7_664 .
Al2 Ce1 Al5 153.95(2) 1_554 .
Al2 Ce1 Al5 94.716(17) . .
Al5 Ce1 Al5 79.20(2) 1_554 .
Al1 Ce1 Al3 148.73(2) 7_665 1_554
Al1 Ce1 Al3 92.646(17) 7_664 1_554
Al2 Ce1 Al3 58.86(2) 1_554 1_554
Al2 Ce1 Al3 106.90(2) . 1_554
Al5 Ce1 Al3 50.44(2) 1_554 1_554
Al5 Ce1 Al3 99.64(2) . 1_554
Al1 Ce1 Al3 92.646(17) 7_665 .
Al1 Ce1 Al3 148.73(2) 7_664 .
Al2 Ce1 Al3 106.90(2) 1_554 .
Al2 Ce1 Al3 58.86(2) . .
Al5 Ce1 Al3 99.64(2) 1_554 .
Al5 Ce1 Al3 50.44(2) . .
Al3 Ce1 Al3 78.24(2) 1_554 .
Al1 Ce1 Al6 140.153(10) 7_665 .
Al1 Ce1 Al6 140.153(10) 7_664 .
Al2 Ce1 Al6 52.824(17) 1_554 .
Al2 Ce1 Al6 52.824(17) . .
Al5 Ce1 Al6 103.63(2) 1_554 .
Al5 Ce1 Al6 103.63(2) . .
Al3 Ce1 Al6 54.110(16) 1_554 .
Al3 Ce1 Al6 54.110(16) . .
Al1 Ce1 Al4 56.46(2) 7_665 .
Al1 Ce1 Al4 104.58(2) 7_664 .
Al2 Ce1 Al4 99.34(2) 1_554 .
Al2 Ce1 Al4 50.11(2) . .
Al5 Ce1 Al4 155.09(2) 1_554 .
Al5 Ce1 Al4 96.131(16) . .
Al3 Ce1 Al4 153.30(2) 1_554 .
Al3 Ce1 Al4 95.819(16) . .
Al6 Ce1 Al4 101.256(18) . .
Al1 Ce1 Al4 104.58(2) 7_665 1_554
Al1 Ce1 Al4 56.46(2) 7_664 1_554
Al2 Ce1 Al4 50.11(2) 1_554 1_554
Al2 Ce1 Al4 99.34(2) . 1_554
Al5 Ce1 Al4 96.131(16) 1_554 1_554
Al5 Ce1 Al4 155.09(2) . 1_554
Al3 Ce1 Al4 95.819(16) 1_554 1_554
Al3 Ce1 Al4 153.30(2) . 1_554
Al6 Ce1 Al4 101.256(18) . 1_554
Al4 Ce1 Al4 77.75(2) . 1_554
Al1 Ce1 Al9 51.330(14) 7_665 3
Al1 Ce1 Al9 51.330(14) 7_664 3
Al2 Ce1 Al9 102.444(18) 1_554 3
Al2 Ce1 Al9 102.444(18) . 3
Al5 Ce1 Al9 103.605(16) 1_554 3
Al5 Ce1 Al9 103.605(16) . 3
Al3 Ce1 Al9 140.574(10) 1_554 3
Al3 Ce1 Al9 140.574(10) . 3
Al6 Ce1 Al9 144.420(15) . 3
Al4 Ce1 Al9 53.326(14) . 3
Al4 Ce1 Al9 53.326(14) 1_554 3
Al9 Co2 Al6 109.78(2) . .
Al9 Co2 Al7 125.42(3) . .
Al6 Co2 Al7 124.80(4) . .
Al9 Co2 Al3 126.522(17) . .
Al6 Co2 Al3 73.23(2) . .
Al7 Co2 Al3 74.37(3) . .
Al9 Co2 Al3 126.522(17) . 1_554
Al6 Co2 Al3 73.23(2) . 1_554
Al7 Co2 Al3 74.37(3) . 1_554
Al3 Co2 Al3 105.93(3) . 1_554
Al9 Co2 Al4 73.39(2) . 3_545
Al6 Co2 Al4 126.785(19) . 3_545
Al7 Co2 Al4 74.39(3) . 3_545
Al3 Co2 Al4 148.76(3) . 3_545
Al3 Co2 Al4 65.43(2) 1_554 3_545
Al9 Co2 Al4 73.39(2) . 3_546
Al6 Co2 Al4 126.785(19) . 3_546
Al7 Co2 Al4 74.39(3) . 3_546
Al3 Co2 Al4 65.43(2) . 3_546
Al3 Co2 Al4 148.76(3) 1_554 3_546
Al4 Co2 Al4 105.50(4) 3_545 3_546
Al9 Co2 Al1 68.55(2) . 1_554
Al6 Co2 Al1 68.96(2) . 1_554
Al7 Co2 Al1 129.052(16) . 1_554
Al3 Co2 Al1 142.19(3) . 1_554
Al3 Co2 Al1 63.27(2) 1_554 1_554
Al4 Co2 Al1 63.32(3) 3_545 1_554
Al4 Co2 Al1 141.94(3) 3_546 1_554
Al9 Co2 Al1 68.55(2) . .
Al6 Co2 Al1 68.96(2) . .
Al7 Co2 Al1 129.052(16) . .
Al3 Co2 Al1 63.27(2) . .
Al3 Co2 Al1 142.19(3) 1_554 .
Al4 Co2 Al1 141.94(3) 3_545 .
Al4 Co2 Al1 63.32(3) 3_546 .
Al1 Co2 Al1 101.90(3) 1_554 .
Al6 Co1 Al8 125.142(8) . .
Al6 Co1 Al8 125.142(8) . 1_554
Al8 Co1 Al8 109.698(16) . 1_554
Al6 Co1 Al7 125.07(3) . 7_565
Al8 Co1 Al7 71.306(15) . 7_565
Al8 Co1 Al7 71.306(15) 1_554 7_565
Al6 Co1 Al7 122.65(3) . 3
Al8 Co1 Al7 71.273(13) . 3
Al8 Co1 Al7 71.273(13) 1_554 3
Al7 Co1 Al7 112.28(2) 7_565 3
Al6 Co1 Al2 70.08(3) . .
Al8 Co1 Al2 63.302(18) . .
Al8 Co1 Al2 145.95(3) 1_554 .
Al7 Co1 Al2 128.584(15) 7_565 .
Al7 Co1 Al2 75.15(3) 3 .
Al6 Co1 Al2 70.08(3) . 1_554
Al8 Co1 Al2 145.95(3) . 1_554
Al8 Co1 Al2 63.302(18) 1_554 1_554
Al7 Co1 Al2 128.584(15) 7_565 1_554
Al7 Co1 Al2 75.15(3) 3 1_554
Al2 Co1 Al2 102.78(3) . 1_554
Al6 Co1 Al5 71.01(2) . 7_564
Al8 Co1 Al5 146.38(3) . 7_564
Al8 Co1 Al5 63.591(16) 1_554 7_564
Al7 Co1 Al5 75.58(3) 7_565 7_564
Al7 Co1 Al5 128.618(17) 3 7_564
Al2 Co1 Al5 141.08(3) . 7_564
Al2 Co1 Al5 63.72(2) 1_554 7_564
Al6 Co1 Al5 71.01(2) . 7_565
Al8 Co1 Al5 63.591(16) . 7_565
Al8 Co1 Al5 146.38(3) 1_554 7_565
Al7 Co1 Al5 75.58(3) 7_565 7_565
Al7 Co1 Al5 128.618(17) 3 7_565
Al2 Co1 Al5 63.72(2) . 7_565
Al2 Co1 Al5 141.08(3) 1_554 7_565
Al5 Co1 Al5 102.74(3) 7_564 7_565
Al6 Co1 Co1 178.76(3) . 5_565
Al8 Co1 Co1 54.849(8) . 5_565
Al8 Co1 Co1 54.849(8) 1_554 5_565
Al7 Co1 Co1 56.17(3) 7_565 5_565
Al7 Co1 Co1 56.11(2) 3 5_565
Al2 Co1 Co1 109.23(3) . 5_565
Al2 Co1 Co1 109.23(3) 1_554 5_565
Al5 Co1 Co1 109.69(2) 7_564 5_565
Al5 Co1 Co1 109.69(2) 7_565 5_565
Al6 Co1 Fe1 178.76(3) . 5_565
Al8 Co1 Fe1 54.849(8) . 5_565
Al8 Co1 Fe1 54.849(8) 1_554 5_565
Al7 Co1 Fe1 56.17(3) 7_565 5_565
Al7 Co1 Fe1 56.11(2) 3 5_565
Al2 Co1 Fe1 109.23(3) . 5_565
Al2 Co1 Fe1 109.23(3) 1_554 5_565
Al5 Co1 Fe1 109.69(2) 7_564 5_565
Al5 Co1 Fe1 109.69(2) 7_565 5_565
Co1 Co1 Fe1 0.000(15) 5_565 5_565
Fe1 Al8 Co1 0.000(18) 5_566 5_566
Fe1 Al8 Co1 180.0 5_566 .
Co1 Al8 Co1 180.0 5_566 .
Fe1 Al8 Fe1 109.698(16) 5_566 5_565
Co1 Al8 Fe1 109.698(16) 5_566 5_565
Co1 Al8 Fe1 70.302(16) . 5_565
Fe1 Al8 Co1 109.698(16) 5_566 5_565
Co1 Al8 Co1 109.698(16) 5_566 5_565
Co1 Al8 Co1 70.302(16) . 5_565
Fe1 Al8 Co1 0.00(2) 5_565 5_565
Fe1 Al8 Co1 70.302(15) 5_566 1_556
Co1 Al8 Co1 70.302(15) 5_566 1_556
Co1 Al8 Co1 109.698(16) . 1_556
Fe1 Al8 Co1 180.000(16) 5_565 1_556
Co1 Al8 Co1 180.000(16) 5_565 1_556
Fe1 Al8 Fe1 70.302(15) 5_566 1_556
Co1 Al8 Fe1 70.302(15) 5_566 1_556
Co1 Al8 Fe1 109.698(16) . 1_556
Fe1 Al8 Fe1 180.000(16) 5_565 1_556
Co1 Al8 Fe1 180.000(16) 5_565 1_556
Co1 Al8 Fe1 0.000(16) 1_556 1_556
Fe1 Al8 Al2 60.454(10) 5_566 5_566
Co1 Al8 Al2 60.454(10) 5_566 5_566
Co1 Al8 Al2 119.546(10) . 5_566
Fe1 Al8 Al2 60.454(10) 5_565 5_566
Co1 Al8 Al2 60.454(10) 5_565 5_566
Co1 Al8 Al2 119.546(10) 1_556 5_566
Fe1 Al8 Al2 119.546(10) 1_556 5_566
Fe1 Al8 Al2 119.546(11) 5_566 .
Co1 Al8 Al2 119.546(11) 5_566 .
Co1 Al8 Al2 60.454(10) . .
Fe1 Al8 Al2 119.546(11) 5_565 .
Co1 Al8 Al2 119.546(11) 5_565 .
Co1 Al8 Al2 60.454(10) 1_556 .
Fe1 Al8 Al2 60.454(10) 1_556 .
Al2 Al8 Al2 180.0 5_566 .
Fe1 Al8 Al5 119.690(10) 5_566 7_565
Co1 Al8 Al5 119.690(10) 5_566 7_565
Co1 Al8 Al5 60.310(10) . 7_565
Fe1 Al8 Al5 119.690(10) 5_565 7_565
Co1 Al8 Al5 119.690(10) 5_565 7_565
Co1 Al8 Al5 60.310(10) 1_556 7_565
Fe1 Al8 Al5 60.310(10) 1_556 7_565
Al2 Al8 Al5 118.28(3) 5_566 7_565
Al2 Al8 Al5 61.72(3) . 7_565
Fe1 Al8 Al5 60.310(10) 5_566 3_556
Co1 Al8 Al5 60.310(10) 5_566 3_556
Co1 Al8 Al5 119.690(10) . 3_556
Fe1 Al8 Al5 60.310(10) 5_565 3_556
Co1 Al8 Al5 60.310(10) 5_565 3_556
Co1 Al8 Al5 119.690(10) 1_556 3_556
Fe1 Al8 Al5 119.690(10) 1_556 3_556
Al2 Al8 Al5 61.72(3) 5_566 3_556
Al2 Al8 Al5 118.28(3) . 3_556
Al5 Al8 Al5 180.0 7_565 3_556
Fe2 Al9 Co2 0.00(2) 5 5
Fe2 Al9 Co2 180.00(2) 5 .
Co2 Al9 Co2 180.00(2) 5 .
Fe2 Al9 Al1 119.935(17) 5 .
Co2 Al9 Al1 119.935(17) 5 .
Co2 Al9 Al1 60.065(17) . .
Fe2 Al9 Al1 60.065(17) 5 5
Co2 Al9 Al1 60.065(17) 5 5
Co2 Al9 Al1 119.935(17) . 5
Al1 Al9 Al1 180.00(3) . 5
Fe2 Al9 Al1 119.935(17) 5 1_554
Co2 Al9 Al1 119.935(17) 5 1_554
Co2 Al9 Al1 60.065(17) . 1_554
Al1 Al9 Al1 92.61(3) . 1_554
Al1 Al9 Al1 87.39(3) 5 1_554
Fe2 Al9 Al1 60.065(17) 5 5_556
Co2 Al9 Al1 60.065(17) 5 5_556
Co2 Al9 Al1 119.935(17) . 5_556
Al1 Al9 Al1 87.39(3) . 5_556
Al1 Al9 Al1 92.61(3) 5 5_556
Al1 Al9 Al1 180.00(4) 1_554 5_556
Fe2 Al9 Al4 56.332(17) 5 7_564
Co2 Al9 Al4 56.332(17) 5 7_564
Co2 Al9 Al4 123.668(17) . 7_564
Al1 Al9 Al4 123.72(2) . 7_564
Al1 Al9 Al4 56.28(2) 5 7_564
Al1 Al9 Al4 63.60(2) 1_554 7_564
Al1 Al9 Al4 116.40(2) 5_556 7_564
Fe2 Al9 Al4 123.668(17) 5 3_546
Co2 Al9 Al4 123.668(17) 5 3_546
Co2 Al9 Al4 56.332(17) . 3_546
Al1 Al9 Al4 56.28(2) . 3_546
Al1 Al9 Al4 123.72(2) 5 3_546
Al1 Al9 Al4 116.40(2) 1_554 3_546
Al1 Al9 Al4 63.60(2) 5_556 3_546
Al4 Al9 Al4 180.00(2) 7_564 3_546
Fe2 Al9 Al4 56.332(17) 5 7_565
Co2 Al9 Al4 56.332(17) 5 7_565
Co2 Al9 Al4 123.668(17) . 7_565
Al1 Al9 Al4 63.60(2) . 7_565
Al1 Al9 Al4 116.40(2) 5 7_565
Al1 Al9 Al4 123.72(2) 1_554 7_565
Al1 Al9 Al4 56.28(2) 5_556 7_565
Al4 Al9 Al4 87.47(2) 7_564 7_565
Al4 Al9 Al4 92.53(2) 3_546 7_565
Fe2 Al9 Al4 123.668(17) 5 3_545
Co2 Al9 Al4 123.668(17) 5 3_545
Co2 Al9 Al4 56.332(17) . 3_545
Al1 Al9 Al4 116.40(2) . 3_545
Al1 Al9 Al4 63.60(2) 5 3_545
Al1 Al9 Al4 56.28(2) 1_554 3_545
Al1 Al9 Al4 123.72(2) 5_556 3_545
Al4 Al9 Al4 92.53(2) 7_564 3_545
Al4 Al9 Al4 87.47(2) 3_546 3_545
Al4 Al9 Al4 180.00(2) 7_565 3_545
Co1 Al2 Fe1 102.78(3) . 1_556
Co1 Al2 Co1 102.78(3) . 1_556
Fe1 Al2 Co1 0.000(14) 1_556 1_556
Co1 Al2 Al8 56.244(18) . .
Fe1 Al2 Al8 56.244(18) 1_556 .
Co1 Al2 Al8 56.244(18) 1_556 .
Co1 Al2 Al4 112.92(3) . .
Fe1 Al2 Al4 112.92(3) 1_556 .
Co1 Al2 Al4 112.92(3) 1_556 .
Al8 Al2 Al4 101.54(4) . .
Co1 Al2 Al5 58.154(18) . 7_565
Fe1 Al2 Al5 58.154(18) 1_556 7_565
Co1 Al2 Al5 58.154(18) 1_556 7_565
Al8 Al2 Al5 59.34(2) . 7_565
Al4 Al2 Al5 160.88(5) . 7_565
Co1 Al2 Al6 50.812(19) . .
Fe1 Al2 Al6 118.87(3) 1_556 .
Co1 Al2 Al6 118.87(3) 1_556 .
Al8 Al2 Al6 102.00(2) . .
Al4 Al2 Al6 127.90(2) . .
Al5 Al2 Al6 61.98(2) 7_565 .
Co1 Al2 Al6 118.87(3) . 1_556
Fe1 Al2 Al6 50.812(19) 1_556 1_556
Co1 Al2 Al6 50.812(19) 1_556 1_556
Al8 Al2 Al6 102.00(2) . 1_556
Al4 Al2 Al6 127.90(2) . 1_556
Al5 Al2 Al6 61.98(2) 7_565 1_556
Al6 Al2 Al6 91.00(4) . 1_556
Co1 Al2 Ce1 167.48(3) . 1_556
Fe1 Al2 Ce1 88.605(9) 1_556 1_556
Co1 Al2 Ce1 88.605(9) 1_556 1_556
Al8 Al2 Ce1 136.131(19) . 1_556
Al4 Al2 Ce1 66.16(2) . 1_556
Al5 Al2 Ce1 126.57(3) 7_565 1_556
Al6 Al2 Ce1 118.97(4) . 1_556
Al6 Al2 Ce1 64.597(19) 1_556 1_556
Co1 Al2 Ce1 88.605(9) . .
Fe1 Al2 Ce1 167.48(3) 1_556 .
Co1 Al2 Ce1 167.48(3) 1_556 .
Al8 Al2 Ce1 136.131(19) . .
Al4 Al2 Ce1 66.16(2) . .
Al5 Al2 Ce1 126.57(3) 7_565 .
Al6 Al2 Ce1 64.597(19) . .
Al6 Al2 Ce1 118.97(4) 1_556 .
Ce1 Al2 Ce1 79.617(19) 1_556 .
Fe1 Al5 Co1 0.00(2) 7_665 7_665
Fe1 Al5 Fe1 102.74(3) 7_665 7_666
Co1 Al5 Fe1 102.74(3) 7_665 7_666
Fe1 Al5 Co1 102.74(3) 7_665 7_666
Co1 Al5 Co1 102.74(3) 7_665 7_666
Fe1 Al5 Co1 0.000(16) 7_666 7_666
Fe1 Al5 Al8 56.100(18) 7_665 3_546
Co1 Al5 Al8 56.100(18) 7_665 3_546
Fe1 Al5 Al8 56.100(18) 7_666 3_546
Co1 Al5 Al8 56.100(18) 7_666 3_546
Fe1 Al5 Al3 112.28(3) 7_665 .
Co1 Al5 Al3 112.28(3) 7_665 .
Fe1 Al5 Al3 112.28(3) 7_666 .
Co1 Al5 Al3 112.28(3) 7_666 .
Al8 Al5 Al3 100.71(3) 3_546 .
Fe1 Al5 Al2 58.13(2) 7_665 7_665
Co1 Al5 Al2 58.13(2) 7_665 7_665
Fe1 Al5 Al2 58.13(2) 7_666 7_665
Co1 Al5 Al2 58.13(2) 7_666 7_665
Al8 Al5 Al2 58.94(3) 3_546 7_665
Al3 Al5 Al2 159.65(4) . 7_665
Fe1 Al5 Al6 117.67(4) 7_665 7_666
Co1 Al5 Al6 117.67(4) 7_665 7_666
Fe1 Al5 Al6 50.408(19) 7_666 7_666
Co1 Al5 Al6 50.408(19) 7_666 7_666
Al8 Al5 Al6 100.87(3) 3_546 7_666
Al3 Al5 Al6 129.54(2) . 7_666
Al2 Al5 Al6 60.77(3) 7_665 7_666
Fe1 Al5 Al6 50.408(19) 7_665 7_665
Co1 Al5 Al6 50.408(19) 7_665 7_665
Fe1 Al5 Al6 117.67(4) 7_666 7_665
Co1 Al5 Al6 117.67(4) 7_666 7_665
Al8 Al5 Al6 100.87(3) 3_546 7_665
Al3 Al5 Al6 129.54(2) . 7_665
Al2 Al5 Al6 60.77(3) 7_665 7_665
Al6 Al5 Al6 89.67(3) 7_666 7_665
Fe1 Al5 Al1 109.19(3) 7_665 7_665
Co1 Al5 Al1 109.19(3) 7_665 7_665
Fe1 Al5 Al1 109.19(3) 7_666 7_665
Co1 Al5 Al1 109.19(3) 7_666 7_665
Al8 Al5 Al1 148.45(4) 3_546 7_665
Al3 Al5 Al1 110.83(4) . 7_665
Al2 Al5 Al1 89.52(4) 7_665 7_665
Al6 Al5 Al1 58.78(2) 7_666 7_665
Al6 Al5 Al1 58.78(2) 7_665 7_665
Fe1 Al5 Ce1 167.78(3) 7_665 1_556
Co1 Al5 Ce1 167.78(3) 7_665 1_556
Fe1 Al5 Ce1 88.935(9) 7_666 1_556
Co1 Al5 Ce1 88.935(9) 7_666 1_556
Al8 Al5 Ce1 135.598(17) 3_546 1_556
Al3 Al5 Ce1 65.40(2) . 1_556
Al2 Al5 Ce1 128.01(2) 7_665 1_556
Al6 Al5 Ce1 67.234(18) 7_666 1_556
Al6 Al5 Ce1 120.79(3) 7_665 1_556
Al1 Al5 Ce1 62.745(19) 7_665 1_556
Fe1 Al5 Ce1 88.935(9) 7_665 .
Co1 Al5 Ce1 88.935(9) 7_665 .
Fe1 Al5 Ce1 167.78(3) 7_666 .
Co1 Al5 Ce1 167.78(3) 7_666 .
Al8 Al5 Ce1 135.598(17) 3_546 .
Al3 Al5 Ce1 65.40(2) . .
Al2 Al5 Ce1 128.01(2) 7_665 .
Al6 Al5 Ce1 120.79(3) 7_666 .
Al6 Al5 Ce1 67.234(18) 7_665 .
Al1 Al5 Ce1 62.745(19) 7_665 .
Ce1 Al5 Ce1 79.20(2) 1_556 .
Co2 Al3 Fe2 105.93(3) . 1_556
Co2 Al3 Co2 105.93(3) . 1_556
Fe2 Al3 Co2 0.00(2) 1_556 1_556
Co2 Al3 Al1 59.65(2) . .
Fe2 Al3 Al1 59.65(2) 1_556 .
Co2 Al3 Al1 59.65(2) 1_556 .
Co2 Al3 Al5 115.96(2) . .
Fe2 Al3 Al5 115.96(2) 1_556 .
Co2 Al3 Al5 115.96(2) 1_556 .
Al1 Al3 Al5 169.57(4) . .
Co2 Al3 Al4 57.41(2) . 3_546
Fe2 Al3 Al4 57.41(2) 1_556 3_546
Co2 Al3 Al4 57.41(2) 1_556 3_546
Al1 Al3 Al4 59.56(3) . 3_546
Al5 Al3 Al4 110.01(4) . 3_546
Co2 Al3 Al6 50.602(19) . .
Fe2 Al3 Al6 118.10(3) 1_556 .
Co2 Al3 Al6 118.10(3) 1_556 .
Al1 Al3 Al6 60.04(2) . .
Al5 Al3 Al6 125.83(2) . .
Al4 Al3 Al6 101.29(3) 3_546 .
Co2 Al3 Al6 118.10(3) . 1_556
Fe2 Al3 Al6 50.602(19) 1_556 1_556
Co2 Al3 Al6 50.602(19) 1_556 1_556
Al1 Al3 Al6 60.04(2) . 1_556
Al5 Al3 Al6 125.83(2) . 1_556
Al4 Al3 Al6 101.29(3) 3_546 1_556
Al6 Al3 Al6 87.67(3) . 1_556
Co2 Al3 Ce1 163.74(3) . 1_556
Fe2 Al3 Ce1 87.286(10) 1_556 1_556
Co2 Al3 Ce1 87.286(10) 1_556 1_556
Al1 Al3 Ce1 123.01(3) . 1_556
Al5 Al3 Ce1 64.158(19) . 1_556
Al4 Al3 Ce1 138.781(14) 3_546 1_556
Al6 Al3 Ce1 114.94(3) . 1_556
Al6 Al3 Ce1 63.108(18) 1_556 1_556
Co2 Al3 Ce1 87.286(10) . .
Fe2 Al3 Ce1 163.74(3) 1_556 .
Co2 Al3 Ce1 163.74(3) 1_556 .
Al1 Al3 Ce1 123.01(3) . .
Al5 Al3 Ce1 64.158(19) . .
Al4 Al3 Ce1 138.781(14) 3_546 .
Al6 Al3 Ce1 63.108(18) . .
Al6 Al3 Ce1 114.94(3) 1_556 .
Ce1 Al3 Ce1 78.24(2) 1_556 .
Fe2 Al4 Co2 0.000(16) 3_556 3_556
Fe2 Al4 Fe2 105.50(4) 3_556 3
Co2 Al4 Fe2 105.50(4) 3_556 3
Fe2 Al4 Co2 105.50(4) 3_556 3
Co2 Al4 Co2 105.50(4) 3_556 3
Fe2 Al4 Co2 0.000(16) 3 3
Fe2 Al4 Al1 59.48(2) 3_556 3_556
Co2 Al4 Al1 59.48(2) 3_556 3_556
Fe2 Al4 Al1 59.48(2) 3 3_556
Co2 Al4 Al1 59.48(2) 3 3_556
Fe2 Al4 Al2 115.74(2) 3_556 .
Co2 Al4 Al2 115.74(2) 3_556 .
Fe2 Al4 Al2 115.74(2) 3 .
Co2 Al4 Al2 115.74(2) 3 .
Al1 Al4 Al2 168.82(5) 3_556 .
Fe2 Al4 Al3 57.16(2) 3_556 3_556
Co2 Al4 Al3 57.16(2) 3_556 3_556
Fe2 Al4 Al3 57.16(2) 3 3_556
Co2 Al4 Al3 57.16(2) 3 3_556
Al1 Al4 Al3 59.35(3) 3_556 3_556
Al2 Al4 Al3 109.46(4) . 3_556
Fe2 Al4 Al9 50.278(12) 3_556 3_556
Co2 Al4 Al9 50.278(12) 3_556 3_556
Fe2 Al4 Al9 117.48(3) 3 3_556
Co2 Al4 Al9 117.48(3) 3 3_556
Al1 Al4 Al9 59.459(19) 3_556 3_556
Al2 Al4 Al9 126.74(2) . 3_556
Al3 Al4 Al9 100.54(3) 3_556 3_556
Fe2 Al4 Al9 117.48(3) 3_556 3
Co2 Al4 Al9 117.48(3) 3_556 3
Fe2 Al4 Al9 50.278(12) 3 3
Co2 Al4 Al9 50.278(12) 3 3
Al1 Al4 Al9 59.459(19) 3_556 3
Al2 Al4 Al9 126.74(2) . 3
Al3 Al4 Al9 100.54(3) 3_556 3
Al9 Al4 Al9 87.47(2) 3_556 3
Fe2 Al4 Ce1 164.13(3) 3_556 .
Co2 Al4 Ce1 164.13(3) 3_556 .
Fe2 Al4 Ce1 87.862(11) 3 .
Co2 Al4 Ce1 87.862(11) 3 .
Al1 Al4 Ce1 123.95(2) 3_556 .
Al2 Al4 Ce1 63.73(2) . .
Al3 Al4 Ce1 138.705(15) 3_556 .
Al9 Al4 Ce1 116.04(3) 3_556 .
Al9 Al4 Ce1 64.613(12) 3 .
Fe2 Al4 Ce1 87.862(11) 3_556 1_556
Co2 Al4 Ce1 87.862(11) 3_556 1_556
Fe2 Al4 Ce1 164.13(3) 3 1_556
Co2 Al4 Ce1 164.13(3) 3 1_556
Al1 Al4 Ce1 123.95(2) 3_556 1_556
Al2 Al4 Ce1 63.73(2) . 1_556
Al3 Al4 Ce1 138.705(15) 3_556 1_556
Al9 Al4 Ce1 64.613(12) 3_556 1_556
Al9 Al4 Ce1 116.04(3) 3 1_556
Ce1 Al4 Ce1 77.75(2) . 1_556
Fe2 Al1 Co2 0.000(19) 1_556 1_556
Fe2 Al1 Co2 101.90(3) 1_556 .
Co2 Al1 Co2 101.90(3) 1_556 .
Fe2 Al1 Al3 57.085(18) 1_556 .
Co2 Al1 Al3 57.085(18) 1_556 .
Co2 Al1 Al3 57.085(18) . .
Fe2 Al1 Al4 57.19(2) 1_556 3_546
Co2 Al1 Al4 57.19(2) 1_556 3_546
Co2 Al1 Al4 57.19(2) . 3_546
Al3 Al1 Al4 61.08(3) . 3_546
Fe2 Al1 Al9 119.93(3) 1_556 .
Co2 Al1 Al9 119.93(3) 1_556 .
Co2 Al1 Al9 51.384(13) . .
Al3 Al1 Al9 105.09(3) . .
Al4 Al1 Al9 64.26(2) 3_546 .
Fe2 Al1 Al9 51.384(13) 1_556 1_556
Co2 Al1 Al9 51.384(13) 1_556 1_556
Co2 Al1 Al9 119.93(3) . 1_556
Al3 Al1 Al9 105.09(3) . 1_556
Al4 Al1 Al9 64.26(2) 3_546 1_556
Al9 Al1 Al9 92.61(3) . 1_556
Fe2 Al1 Al6 51.365(19) 1_556 1_556
Co2 Al1 Al6 51.365(19) 1_556 1_556
Co2 Al1 Al6 119.41(4) . 1_556
Al3 Al1 Al6 63.94(3) . 1_556
Al4 Al1 Al6 105.07(3) 3_546 1_556
Al9 Al1 Al6 168.22(4) . 1_556
Al9 Al1 Al6 86.581(12) 1_556 1_556
Fe2 Al1 Al6 119.41(4) 1_556 .
Co2 Al1 Al6 119.41(4) 1_556 .
Co2 Al1 Al6 51.365(19) . .
Al3 Al1 Al6 63.94(3) . .
Al4 Al1 Al6 105.07(3) 3_546 .
Al9 Al1 Al6 86.581(12) . .
Al9 Al1 Al6 168.22(4) 1_556 .
Al6 Al1 Al6 91.81(3) 1_556 .
Fe2 Al1 Al5 111.93(3) 1_556 7_565
Co2 Al1 Al5 111.93(3) 1_556 7_565
Co2 Al1 Al5 111.93(3) . 7_565
Al3 Al1 Al5 95.96(4) . 7_565
Al4 Al1 Al5 157.04(4) 3_546 7_565
Al9 Al1 Al5 127.55(2) . 7_565
Al9 Al1 Al5 127.55(2) 1_556 7_565
Al6 Al1 Al5 60.58(2) 1_556 7_565
Al6 Al1 Al5 60.58(2) . 7_565
Fe2 Al1 Ce1 168.89(3) 1_556 7_565
Co2 Al1 Ce1 168.89(3) 1_556 7_565
Co2 Al1 Ce1 89.203(8) . 7_565
Al3 Al1 Ce1 131.77(2) . 7_565
Al4 Al1 Ce1 131.02(2) 3_546 7_565
Al9 Al1 Ce1 66.900(11) . 7_565
Al9 Al1 Ce1 122.29(3) 1_556 7_565
Al6 Al1 Ce1 123.14(3) 1_556 7_565
Al6 Al1 Ce1 68.060(18) . 7_565
Al5 Al1 Ce1 63.33(2) 7_565 7_565
Co2 Al7 Fe1 146.07(5) . 7_665
Co2 Al7 Co1 146.07(5) . 7_665
Fe1 Al7 Co1 0.000(18) 7_665 7_665
Co2 Al7 Co1 146.21(5) . 3_545
Fe1 Al7 Co1 67.72(2) 7_665 3_545
Co1 Al7 Co1 67.72(2) 7_665 3_545
Co2 Al7 Fe1 146.21(5) . 3_545
Fe1 Al7 Fe1 67.72(2) 7_665 3_545
Co1 Al7 Fe1 67.72(2) 7_665 3_545
Co1 Al7 Fe1 0.000(17) 3_545 3_545
Co2 Al7 Al8 136.382(11) . 3_546
Fe1 Al7 Al8 53.054(13) 7_665 3_546
Co1 Al7 Al8 53.054(13) 7_665 3_546
Co1 Al7 Al8 53.039(15) 3_545 3_546
Fe1 Al7 Al8 53.039(15) 3_545 3_546
Co2 Al7 Al8 136.382(11) . 3_545
Fe1 Al7 Al8 53.054(13) 7_665 3_545
Co1 Al7 Al8 53.054(13) 7_665 3_545
Co1 Al7 Al8 53.039(15) 3_545 3_545
Fe1 Al7 Al8 53.039(15) 3_545 3_545
Al8 Al7 Al8 87.24(2) 3_546 3_545
Co1 Al6 Co2 178.03(4) . .
Co1 Al6 Al1 119.22(3) . 1_554
Co2 Al6 Al1 59.67(2) . 1_554
Co1 Al6 Al1 119.22(3) . .
Co2 Al6 Al1 59.67(2) . .
Al1 Al6 Al1 91.81(3) 1_554 .
Co1 Al6 Al2 59.11(2) . .
Co2 Al6 Al2 121.97(3) . .
Al1 Al6 Al2 178.18(4) 1_554 .
Al1 Al6 Al2 88.57(2) . .
Co1 Al6 Al2 59.11(2) . 1_554
Co2 Al6 Al2 121.97(3) . 1_554
Al1 Al6 Al2 88.57(2) 1_554 1_554
Al1 Al6 Al2 178.18(4) . 1_554
Al2 Al6 Al2 91.00(4) . 1_554
Co1 Al6 Al5 58.58(2) . 7_564
Co2 Al6 Al5 120.29(3) . 7_564
Al1 Al6 Al5 60.64(2) 1_554 7_564
Al1 Al6 Al5 121.50(4) . 7_564
Al2 Al6 Al5 117.69(3) . 7_564
Al2 Al6 Al5 57.24(2) 1_554 7_564
Co1 Al6 Al5 58.58(2) . 7_565
Co2 Al6 Al5 120.29(3) . 7_565
Al1 Al6 Al5 121.50(4) 1_554 7_565
Al1 Al6 Al5 60.64(2) . 7_565
Al2 Al6 Al5 57.24(2) . 7_565
Al2 Al6 Al5 117.69(3) 1_554 7_565
Al5 Al6 Al5 89.67(3) 7_564 7_565
Co1 Al6 Al3 124.90(2) . .
Co2 Al6 Al3 56.17(2) . .
Al1 Al6 Al3 115.85(3) 1_554 .
Al1 Al6 Al3 56.02(2) . .
Al2 Al6 Al3 65.80(2) . .
Al2 Al6 Al3 125.32(3) 1_554 .
Al5 Al6 Al3 176.17(4) 7_564 .
Al5 Al6 Al3 91.21(2) 7_565 .
Co1 Al6 Al3 124.90(2) . 1_554
Co2 Al6 Al3 56.17(2) . 1_554
Al1 Al6 Al3 56.02(2) 1_554 1_554
Al1 Al6 Al3 115.85(3) . 1_554
Al2 Al6 Al3 125.32(3) . 1_554
Al2 Al6 Al3 65.80(2) 1_554 1_554
Al5 Al6 Al3 91.21(2) 7_564 1_554
Al5 Al6 Al3 176.17(4) 7_565 1_554
Al3 Al6 Al3 87.67(3) . 1_554
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ce1 Al1 3.1402(7) 7_665
Ce1 Al1 3.1402(7) 7_664
Ce1 Al2 3.1427(6) 1_554
Ce1 Al2 3.1427(6) .
Ce1 Al5 3.1564(7) 1_554
Ce1 Al5 3.1564(7) .
Ce1 Al3 3.1889(7) 1_554
Ce1 Al3 3.1889(7) .
Ce1 Al6 3.1982(8) .
Ce1 Al4 3.2058(8) .
Ce1 Al4 3.2058(8) 1_554
Ce1 Al9 3.27835(18) 3
Co2 Al9 2.3360(4) .
Co2 Al6 2.3447(9) .
Co2 Al7 2.4655(9) .
Co2 Al3 2.5205(6) .
Co2 Al3 2.5205(6) 1_554
Co2 Al4 2.5277(6) 3_545
Co2 Al4 2.5277(6) 3_546
Co2 Al1 2.5909(6) 1_554
Co2 Al1 2.5909(6) .
Co1 Al6 2.3257(9) .
Co1 Al8 2.4608(2) .
Co1 Al8 2.4608(2) 1_554
Co1 Al7 2.5418(9) 7_565
Co1 Al7 2.5438(10) 3
Co1 Al2 2.5749(5) .
Co1 Al2 2.5749(5) 1_554
Co1 Al5 2.5756(6) 7_564
Co1 Al5 2.5756(6) 7_565
Co1 Co1 2.8336(8) 5_565
Co1 Fe1 2.8336(8) 5_565
Al8 Fe1 2.4608(2) 5_566
Al8 Co1 2.4608(2) 5_566
Al8 Fe1 2.4608(2) 5_565
Al8 Co1 2.4608(2) 5_565
Al8 Co1 2.4608(2) 1_556
Al8 Fe1 2.4608(2) 1_556
Al8 Al2 2.6443(9) 5_566
Al8 Al2 2.6443(9) .
Al8 Al5 2.6554(8) 7_565
Al8 Al5 2.6554(8) 3_556
Al9 Fe2 2.3360(4) 5
Al9 Co2 2.3360(4) 5
Al9 Al1 2.7827(6) .
Al9 Al1 2.7827(6) 5
Al9 Al1 2.7827(6) 1_554
Al9 Al1 2.7827(6) 5_556
Al9 Al4 2.9104(6) 7_564
Al9 Al4 2.9104(6) 3_546
Al9 Al4 2.9104(6) 7_565
Al9 Al4 2.9104(6) 3_545
Al2 Fe1 2.5749(5) 1_556
Al2 Co1 2.5749(5) 1_556
Al2 Al4 2.6891(13) .
Al2 Al5 2.7185(12) 7_565
Al2 Al6 2.8210(9) .
Al2 Al6 2.8210(9) 1_556
Al2 Ce1 3.1427(6) 1_556
Al5 Fe1 2.5756(6) 7_665
Al5 Co1 2.5756(6) 7_665
Al5 Fe1 2.5756(6) 7_666
Al5 Co1 2.5756(6) 7_666
Al5 Al8 2.6554(8) 3_546
Al5 Al3 2.7039(14) .
Al5 Al2 2.7185(12) 7_665
Al5 Al6 2.8537(8) 7_666
Al5 Al6 2.8537(8) 7_665
Al5 Al1 2.8551(12) 7_665
Al5 Ce1 3.1564(7) 1_556
Al3 Fe2 2.5205(6) 1_556
Al3 Co2 2.5205(6) 1_556
Al3 Al1 2.6816(13) .
Al3 Al4 2.7282(13) 3_546
Al3 Al6 2.9051(8) .
Al3 Al6 2.9051(8) 1_556
Al3 Ce1 3.1889(7) 1_556
Al4 Fe2 2.5277(6) 3_556
Al4 Co2 2.5277(6) 3_556
Al4 Fe2 2.5277(6) 3
Al4 Co2 2.5277(6) 3
Al4 Al1 2.6874(13) 3_556
Al4 Al3 2.7282(13) 3_556
Al4 Al9 2.9104(6) 3_556
Al4 Al9 2.9104(6) 3
Al4 Ce1 3.2058(8) 1_556
Al1 Fe2 2.5909(6) 1_556
Al1 Co2 2.5909(6) 1_556
Al1 Al4 2.6874(13) 3_546
Al1 Al9 2.7827(6) 1_556
Al1 Al6 2.8015(8) 1_556
Al1 Al6 2.8015(8) .
Al1 Al5 2.8551(12) 7_565
Al1 Ce1 3.1402(7) 7_565
Al7 Fe1 2.5418(9) 7_665
Al7 Co1 2.5418(9) 7_665
Al7 Co1 2.5438(10) 3_545
Al7 Fe1 2.5438(10) 3_545
Al7 Al8 2.9167(6) 3_546
Al7 Al8 2.9167(6) 3_545
Al6 Al1 2.8015(8) 1_554
Al6 Al2 2.8210(9) 1_554
Al6 Al5 2.8537(8) 7_564
Al6 Al5 2.8537(8) 7_565
Al6 Al3 2.9051(8) 1_554
